Presentation on theme: "Chapter 13 - 1 Chapter 13: Applications and Processing of Ceramics ISSUES TO ADDRESS... How do we classify ceramics ? What are some applications of ceramics."— Presentation transcript:
Chapter Chapter 13: Applications and Processing of Ceramics ISSUES TO ADDRESS... How do we classify ceramics ? What are some applications of ceramics ? How is processing of ceramics different than for metals ?
Chapter GlassesClay products RefractoriesAbrasivesCementsAdvanced ceramics -optical -composite reinforce -containers/ household -whiteware -structural -bricks for high T (furnaces) -sandpaper -cutting -polishing -composites -structural -engine rotors valves bearings -sensors Adapted from Fig and discussion in Section , Callister & Rethwisch 8e. Classification of Ceramics Ceramic Materials
Chapter tensile force A o A d die Die blanks: -- Need wear resistant properties! Die surface: -- 4 m polycrystalline diamond particles that are sintered onto a cemented tungsten carbide substrate. -- polycrystalline diamond gives uniform hardness in all directions to reduce wear. Adapted from Fig. 11.8(d), Callister & Rethwisch 8e. Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission. Ceramics Application: Die Blanks
Chapter Tools: -- for grinding glass, tungsten, carbide, ceramics -- for cutting Si wafers -- for oil drilling blades oil drill bits Single crystal diamonds polycrystalline diamonds in a resin matrix. Photos courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission. Ceramics Application: Cutting Tools Materials: -- manufactured single crystal or polycrystalline diamonds in a metal or resin matrix. -- polycrystalline diamonds resharpen by microfracturing along cleavage planes.
Chapter Example: ZrO 2 as an oxygen sensor Principle: Increase diffusion rate of oxygen to produce rapid response of sensor signal to change in oxygen concentration Ceramics Application: Sensors A substituting Ca 2+ ion removes a Zr 4+ ion and an O 2- ion. Ca 2+ Approach: Add Ca impurity to ZrO 2 : -- increases O 2- vacancies -- increases O 2- diffusion rate reference gas at fixed oxygen content O 2- diffusion gas with an unknown, higher oxygen content - + voltage difference produced! sensor Operation: -- voltage difference produced when O 2- ions diffuse from the external surface through the sensor to the reference gas surface. -- magnitude of voltage difference partial pressure of oxygen at the external surface
Chapter Materials to be used at high temperatures (e.g., in high temperature furnaces). Consider the Silica (SiO 2 ) - Alumina (Al 2 O 3 ) system. Silica refractories - silica rich - small additions of alumina depress melting temperature (phase diagram): Fig , Callister & Rethwisch 8e. (Fig adapted from F.J. Klug and R.H. Doremus, J. Am. Cer. Soc. 70(10), p. 758, 1987.) Refractories Composition (wt% alumina) T(ºC) alumina + mullite + L mullite Liquid (L)(L) mullite +crystobalite + L alumina + L 3Al 2 O 3 -2SiO 2
Chapter Advanced Ceramics: Materials for Automobile Engines Advantages: –Operate at high temperatures – high efficiencies –Low frictional losses –Operate without a cooling system –Lower weights than current engines Disadvantages: –Ceramic materials are brittle –Difficult to remove internal voids (that weaken structures) –Ceramic parts are difficult to form and machine Potential candidate materials: Si 3 N 4, SiC, & ZrO 2 Possible engine parts: engine block & piston coatings
Chapter Advanced Ceramics: Materials for Ceramic Armor Components: -- Outer facing plates -- Backing sheet Properties/Materials: -- Facing plates -- hard and brittle — fracture high-velocity projectile — Al 2 O 3, B 4 C, SiC, TiB 2 -- Backing sheets -- soft and ductile — deform and absorb remaining energy — aluminum, synthetic fiber laminates
Chapter Blowing of Glass Bottles: GLASS FORMING Adapted from Fig. 13.8, Callister & Rethwisch 8e. (Fig is adapted from C.J. Phillips, Glass: The Miracle Maker, Pittman Publishing Ltd., London.) Ceramic Fabrication Methods (i) Gob Parison mold Pressing operation Suspended parison Finishing mold Compressed air Fiber drawing: wind up PARTICULATE FORMING CEMENTATION -- glass formed by application of pressure -- mold is steel with graphite lining Pressing: plates, cheap glasses
Chapter Sheet Glass Forming Sheet forming – continuous casting –sheets are formed by floating the molten glass on a pool of molten tin Adapted from Fig. 13.9, Callister & Rethwisch 8e.
Chapter Quartz is crystalline SiO 2 : Basic Unit: Glass is noncrystalline (amorphous) Fused silica is SiO 2 to which no impurities have been added Other common glasses contain impurity ions such as Na +, Ca 2+, Al 3+, and B 3+ (soda glass) Adapted from Fig , Callister & Rethwisch 8e. Glass Structure Si0 4 tetrahedron 4- Si 4+ O 2- Si 4+ Na + O 2-
Chapter Specific volume (1 ) vs Temperature (T): Glasses: -- do not crystallize -- change in slope in spec. vol. curve at glass transition temperature, T g -- transparent - no grain boundaries to scatter light Crystalline materials: -- crystallize at melting temp, T m -- have abrupt change in spec. vol. at T m Adapted from Fig. 13.6, Callister & Rethwisch 8e. Glass Properties T Specific volume Supercooled Liquid solid TmTm Liquid (disordered) Crystalline (i.e., ordered) TgTg Glass (amorphous solid)
Chapter Glass Properties: Viscosity Viscosity, : -- relates shear stress ( ) and velocity gradient (dv/dy): has units of (Pa-s) velocity gradient dvdv dydy glass dvdv dydy
Chapter Viscosity [Pa-s] T(ºC) Working range: glass-forming carried out annealing point T melt strain point Viscosity decreases with T Adapted from Fig. 13.7, Callister & Rethwisch 8e. (Fig is from E.B. Shand, Engineering Glass, Modern Materials, Vol. 6, Academic Press, New York, 1968, p. 262.) Log Glass Viscosity vs. Temperature fused silica: > 99.5 wt% SiO 2 soda-lime glass: 70% SiO 2 balance Na 2 O (soda) & CaO (lime) Vycor: 96% SiO 2, 4% B 2 O 3 borosilicate (Pyrex): 13% B 2 O 3, 3.5% Na 2 O, 2.5% Al 2 O 3 soda-lime glass 96% silica fused silica Pyrex
Chapter Annealing: -- removes internal stresses caused by uneven cooling. Tempering: -- puts surface of glass part into compression -- suppresses growth of cracks from surface scratches. -- sequence: Heat Treating Glass at room temp. tension compression before cooling hot initial cooling hot cooler -- Result: surface crack growth is suppressed.
Chapter Mill (grind) and screen constituents: desired particle size Extrude this mass (e.g., into a brick) Dry and fire the formed piece ram billet container force die holder die A o A d extrusion Adapted from Fig. 12.8(c), Callister & Rethwisch 8e. Ceramic Fabrication Methods (iia) GLASS FORMING PARTICULATE FORMING CEMENTATION Hydroplastic forming:
Chapter Mill (grind) and screen constituents: desired particle size Slip casting operation Dry and fire the cast piece Ceramic Fabrication Methods (iia) solid component Adapted from Fig , Callister & Rethwisch 8e. (Fig is from W.D. Kingery, Introduction to Ceramics, John Wiley and Sons, Inc., 1960.) hollow component pour slip into mold drain mold “green ceramic” pour slip into mold absorb water into mold “green ceramic” GLASS FORMING PARTICULATE FORMING CEMENTATION Slip casting: Mix with water and other constituents to form slip
Chapter Typical Porcelain Composition (50%) 1. Clay (25%) 2. Filler – e.g. quartz (finely ground) (25%) 3. Fluxing agent (Feldspar) -- aluminosilicates plus K +, Na +, Ca + -- upon firing - forms low-melting-temp. glass
Chapter Clay is inexpensive When water is added to clay -- water molecules fit in between layered sheets -- reduces degree of van der Waals bonding -- when external forces applied – clay particles free to move past one another – becomes hydroplastic Structure of Kaolinite Clay: Adapted from Fig , Callister & Rethwisch 8e. (Fig is adapted from W.E. Hauth, "Crystal Chemistry of Ceramics", American Ceramic Society Bulletin, Vol. 30 (4), 1951, p. 140.) Hydroplasticity of Clay weak van der Waals bonding charge neutral charge neutral Si 4+ Al 3+ - OH O 2- Shear
Chapter Drying : as water is removed - interparticle spacings decrease – shrinkage. Adapted from Fig , Callister & Rethwisch 8e. (Fig is from W.D. Kingery, Introduction to Ceramics, John Wiley and Sons, Inc., 1960.) Drying and Firing Drying too fast causes sample to warp or crack due to non-uniform shrinkage wet body partially drycompletely dry Firing : -- heat treatment between ºC -- vitrification: liquid glass forms from clay and flux – flows between SiO 2 particles. (Flux lowers melting temperature). Adapted from Fig , Callister & Rethwisch 8e. (Fig is courtesy H.G. Brinkies, Swinburne University of Technology, Hawthorn Campus, Hawthorn, Victoria, Australia.) Si0 2 particle (quartz) glass formed around the particle micrograph of porcelain 70 m
Chapter Powder Pressing: used for both clay and non-clay compositions. Powder (plus binder) compacted by pressure in a mold -- Uniaxial compression - compacted in single direction -- Isostatic (hydrostatic) compression - pressure applied by fluid - powder in rubber envelope -- Hot pressing - pressure + heat ( Ceramic Fabrication Methods (iib) GLASS FORMING PARTICULATE FORMING CEMENTATION
Chapter Sintering Adapted from Fig , Callister & Rethwisch 8e. Aluminum oxide powder: -- sintered at 1700ºC for 6 minutes. Adapted from Fig , Callister & Rethwisch 8e. (Fig is from W.D. Kingery, H.K. Bowen, and D.R. Uhlmann, Introduction to Ceramics, 2nd ed., John Wiley and Sons, Inc., 1976, p. 483.) 15 m Sintering occurs during firing of a piece that has been powder pressed -- powder particles coalesce and reduction of pore size
Chapter Tape Casting Thin sheets of green ceramic cast as flexible tape Used for integrated circuits and capacitors Slip = suspended ceramic particles + organic liquid (contains binders, plasticizers) Fig , Callister & Rethwisch 8e.
Chapter Hardening of a paste – paste formed by mixing cement material with water Formation of rigid structures having varied and complex shapes Hardening process – hydration (complex chemical reactions involving water and cement particles) Ceramic Fabrication Methods (iii) GLASS FORMING PARTICULATE FORMING CEMENTATION Portland cement – production of: -- mix clay and lime-bearing minerals -- calcine (heat to 1400ºC) -- grind into fine powder